Text of Replacement Macgregor 26M dagger board fabrication: by ... · PDF file Replacement Macgregor...
Z:\Mikes\Year 2018\Tarka 2018\Dagger1\The Dagger board instructions 3a final docx.docx.17/08/18 1
Replacement Macgregor 26M dagger board fabrication: by Mike Clarke 19/08/18
Fabricating a new hollow section dagger board requires three main processes:
1) Lay up two side sections in a mould (2 days)
2) Bond the two sides together with a stiffening rib (1 day)
3) Seal the edges and make good the gel coat (2 days)
Assuming you already have a mould.
We broke the dagger-board on Tarka our Macgregor 26M three weeks ago – a new dagger-board from the
USA costs $550 plus $280 package and then UK VAT and import duty so it’s expensive at just over £1,000 and
several weeks delivery time.
I posted a note on the website to see if anyone had a spare dagger board and was pleasantly surprised to
find that Simon Armitage not only had a spare but it was only an hour’s drive away at Bradwell Marina. So
off we went to collect it. It turned out to have had a repair at some time that Simon was not aware of but
after a day grinding off the surface coatings and rubbing it down back to the original gelcoat and making good
the repaired section it looked OK. I checked inside it with an endoscope to see if there was any structural
damage and it looked OK so it got a coat of two pack Hempel epoxy gel coat protect paint and was installed
as at least a temporary fix to get us sailing again.
I then decided to attempt to make a new dagger-board by taking a mould from the old damaged one. It
should only need a single mould of one side as the board is symmetrical end to end. Making this turned out
to be a bigger job than first anticipated mostly due to the amount of time it took to repair and make good
the damage to the old dagger board ready to take a mould from. I first made good the damage by cutting out
a section from the worst damaged side and laying up some fibre glass matt against the inside of the less
damaged side. This gave me a surface to fill against and make the shape right using polyester filler (plastic
padding in the first instance, although I later found there are better and cheaper gel coat putty fillers available
on-line). I used the shape of the undamaged surrounding area to ensure the repaired part had the same
profile. This entailed multiple filling and rubbing down sessions but eventually it was about right. I then used
two coats of Durabuild surface primer which is a two part high build polymer specifically for mould formers.
This allowed me to rub the surface down to a uniform finish suitable to take the mould release agent. I then
made up a wooden frame round the entire board set it at little over half way down the thickness of the board.
I hot melt glued this to the edge of the board to fill in the inevitable small gaps to prevent the gel coat dripping
through. This frame gave a flange that could later be cut off with the rough edges. I put masking tape round
the outside edge of the frame to create a slight stand up edge so that the gel coat and glass resin didn’t run
off onto the floor when laying up.
It turns out that the dagger board is almost exactly one square meter per side so a 1m2 mould making Kit
from East Coast Fibreglass Supplies was used to make the mould. The process for making the mould was:
1. Polish the former that the mould is going to be taken from i.e. the old half repaired dagger-board.
2. Rub in twelve, yes twelve, layers of mould release wax polish allowing to dry for at least 20 min
between coats. This is necessary to ensure the moulding gel coat can release; you really don’t want
it to stick!
3. Paint on a thin layer of PVA mould release and allow to dry immediately before applying the gel-coat.
4. Paint on a thick layer – pour and spread more than paint – a layer of the thixotropic special mould
gel coat. A thick green gunge that starts to gel very quickly in the warm weather we were having –
don’t overwork it!
5. Once the gel coat had set after about 2 hours, I added a thin layer of 300gm-2 chopped strand mat
(csm) wetted on with a vinyl ester moulding resin (part of the kit).
6. When this had set overnight I added four layers of 450gm-2 chopped strand glass mat using Optimould
moulding resin. This is a special resin for making moulds that doesn’t shrink or distort as it sets – but
it does get very hot as it must get above 40°C to properly cure and turn it an off white colour.
7. After this had set overnight I glassed in a wooden batten along the leading (thick) edge and cut out
and glassed in four pieces of wood to stiffen and support the mould. This was then left for two days
Z:\Mikes\Year 2018\Tarka 2018\Dagger1\The Dagger board instructions 3a final docx.docx.17/08/18 2
After two days I thought it must have cured in the warm weather we had as it was up in the 30’s both days,
so I trimmed the rough edges through to the wooden battens with a cutting disc and gently eased the mould
off the core, which once started came away quite easily.
At this point I took the opportunity to cut some more sections out of the unrepaired side of the original
dagger board to better see its internal structure and how it had been built. It appears that the board was
built by moulding the two sides in vinyl ester resin with a gel coat, a thin chopped glass mat and a heavy glass
mat followed by two layers of woven glass cloth for the main surface of the sides. This gave about a 3mm
thick skin which was thicker in the reinforced longitudinal section and at the edges. There is a moulded in,
structural hollow section down the centre that was laid up on a foam core so that when it was still wet it
could be deformed and bond to the other side of the moulding when the two sides were pushed together.
The edges and ends appear to have been flooded with resin that was allowed to set to give a thick section to
all the edges. This is what I tried to replicate using the new mould.
I used a vinyl ester resin (Crystic VE 679pa supplied by East Coast Fibreglass Supplies) rather than a polyester
resin as the US web site claims that the new boards are made with this. This makes sense as the cheaper
polyester resins are not as strong and are not as resistant to continues water immersion. East Coast Fibreglass
Supplies also has a website with useful articles on how to use their products. I considered using epoxy resin
but it is much harder to work with to make a good strong section, is more likely to delaminate under flexing
and only marginally stronger than vinyl ester whilst being considerably more expensive. The lower end of the
dagger-board is continually immersed for the first 200mm if the boat is kept in the water with the board up
as ours is. The internal space is always wet as it is flooded in use and unlikely to ever completely dry out
especially with foam core in the stiffened section absorbing water when it’s used.
The assembly of the two halves was always going to be something of a challenge as not only do the two sides
have to match up but they have to be assembled with the centre reinforced rib still wet enough to be
deformed into place against the upper side. But first the two side sections need to be moulded.
Laying up sections in mould:
First some Elf’ and safety:
Acetone, catalyst and resin fumes and liquids are flammable – don’t have any flames in area.
The fumes of these materials are not good for you so use a respirator fitted with a carbon filter when laying
up the resin.
DO NOT SMOKE in the area at any time as any fumes sucked through a cigarettes are especially toxic and you
may well start a fire or explosion with any vapours present.
Glass fibre dust is a severe eye and respiratory irritant so use a dust mask and eye protection when cutting,
grinding or sanding.
Wear eye protection especially when using resin catalyst as it is a strong oxidising agent and splashes can
damage eyes. (Have an eyewash bottle or water available for emergencies)
Wear disposable nitrile gloves as resin doesn’t wash off with soap and water and is a skin irritant.
Each side was fabricated by laying up the glass fibre and resin in the mould in the same way:
1) Make good and damage to the masking tape wrapped over the edge of the mould. The top surface
must then be re-waxed to prevent the gel coat sticking but keep the side free of wax allow a second
stand up edge of tape to be applied in step 4 below.
2) The Four coats of release wax applied at 20 min intervals – it’s not a polish - the intention is to ensure
all the surface is covered with a good layer of wax and all the pores, small holes and imperfections
are filled with the wax; so it’s important that at least four layers are applied, no shortcuts here or
you can destroy both the mould and the moulded part. It’s a lot easier to apply wax than repair the
3) When the last coat of release wax had dried a thin coat of PVA release agent was applied using a
foam pad brush or sponge to give a thin but continuous film. This was allowed to dry.
4) The edges of the mould were built up with masking tape to stop the gel coat dripping off. Six hundred
and fifty grams of gel coat was weighed out (kitchen scales in a clear plastic bag to protect it) into a
polyethylene paint pot and catalysed with 2% (13g) of MEKP. This needs to be very well mixed with
Z:\Mikes\Year 2018\Tarka 2018\Dagger1\The Dagger board instructions 3a final docx.docx.17/08/18 3
a wooden stirrer but as it goes off in about 15 minutes at 20°C so you can’t hang about. It can then
be poured into the mould and spread with a short hair roller and a 1” brush making sure the whole
area is covered with a